multilayer ceramic capacitors/axial & ceramic capacitors/axial & radial leaded multilayer ceramic...
Post on 27-Jun-2018
Embed Size (px)
KEMET Electronics Corporation, P.O. Box 5928, Greenville, S.C. 29606, (864) 963-63004
MULTILAYER CERAMIC CAPACITORS/AXIAL & RADIAL LEADED
Multilayer ceramic capacitors are available in avariety of physical sizes and configurations, includingleaded devices and surface mounted chips. Leadedstyles include molded and conformally coated partswith axial and radial leads. However, the basiccapacitor element is similar for all styles. It is called achip and consists of formulated dielectric materialswhich have been cast into thin layers, interspersedwith metal electrodes alternately exposed on opposite
edges of the laminated structure. The entire structure isfired at high temperature to produce a monolithicblock which provides high capacitance values in asmall physical volume. After firing, conductiveterminations are applied to opposite ends of the chip tomake contact with the exposed electrodes.Termination materials and methods vary depending onthe intended use.
TEMPERATURE CHARACTERISTICSCeramic dielectric materials can be formulated with
a wide range of characteristics. The EIA standard forceramic dielectric capacitors (RS-198) divides ceramicdielectrics into the following classes:
Class I: Temperature compensating capacitors,suitable for resonant circuit application or other appli-cations where high Q and stability of capacitance char-acteristics are required. Class I capacitors havepredictable temperature coefficients and are notaffected by voltage, frequency or time. They are madefrom materials which are not ferro-electric, yieldingsuperior stability but low volumetric efficiency. Class Icapacitors are the most stable type available, but havethe lowest volumetric efficiency.
Class II: Stable capacitors, suitable for bypassor coupling applications or frequency discriminatingcircuits where Q and stability of capacitance char-acteristics are not of major importance. Class IIcapacitors have temperature characteristics of 15%or less. They are made from materials which areferro-electric, yielding higher volumetric efficiency butless stability. Class II capacitors are affected bytemperature, voltage, frequency and time.
Class III: General purpose capacitors, suitablefor by-pass coupling or other applications in whichdielectric losses, high insulation resistance andstability of capacitance characteristics are of little orno importance. Class III capacitors are similar to ClassII capacitors except for temperature characteristics,which are greater than 15%. Class III capacitorshave the highest volumetric efficiency and pooreststability of any type.
KEMET leaded ceramic capacitors are offered inthe three most popular temperature characteristics:
C0G: Class I, with a temperature coefficient of 0 30 ppm per degree C over an operatingtemperature range of - 55C to + 125C (Alsoknown as NP0).X7R: Class II, with a maximum capacitancechange of 15% over an operating temperaturerange of - 55C to + 125C.Z5U: Class III, with a maximum capacitancechange of + 22% - 56% over an operating tem-perature range of + 10C to + 85C.
Specified electrical limits for these three temperaturecharacteristics are shown in Table 1.
SPECIFIED ELECTRICAL LIMITS
C0G X7R Z5U
Dissipation Factor: Measured at following conditions.C0G 1 kHz and 1 vrms if capacitance >1000pF
1 MHz and 1 vrms if capacitance 1000 pFX7R 1 kHz and 1 vrms* or if extended cap range 0.5 vrmsZ5U 1 kHz and 0.5 vrms
0.10% 2.5%(3.5% @ 25V) 4.0%
Dielectric Stength: 2.5 times rated DC voltage.
Insulation Resistance (IR): At rated DC voltage,whichever of the two is smaller
1,000 M For 100 G
1,000 M For 100 G
1,000 M For 10 G
Temperature Characteristics: Range, CCapacitance Change withoutDC voltage
-55 to +1250 30 ppm/C
-55 to +125 15%
+ 10 to +85+22%,-56%
* MHz and 1 vrms if capacitance 100 pF on military product.
Parameter Temperature Characteristics
Pass Subsequent IR Test
The fundamental electrical properties of multilayerceramic capacitors are as follows:
Polarity: Multilayer ceramic capacitors are not polar,and may be used with DC voltage applied in either direction.
Rated Voltage: This term refers to the maximum con-tinuous DC working voltage permissible across the entireoperating temperature range. Multilayer ceramic capacitorsare not extremely sensitive to voltage, and brief applicationsof voltage above rated will not result in immediate failure.However, reliability will be reduced by exposure to sustainedvoltages above rated.
Capacitance: The standard unit of capacitance is thefarad. For practical capacitors, it is usually expressed inmicrofarads (10-6 farad), nanofarads (10-9 farad), or picofarads(10-12 farad). Standard measurement conditions are asfollows:
Class I (up to 1,000 pF): 1MHz and 1.2 VRMSmaximum.
Class I (over 1,000 pF): 1kHz and 1.2 VRMSmaximum.
Class II: 1 kHz and 1.0 0.2 VRMS.
Class III: 1 kHz and 0.5 0.1 VRMS.
Like all other practical capacitors, multilayer ceramiccapacitors also have resistance and inductance. A simplifiedschematic for the equivalent circuit is shown in Figure 1.Other significant electrical characteristics resulting fromthese additional properties are as follows:
Impedance: Since the parallel resistance (Rp) is nor-mally very high, the total impedance of the capacitor is:
C = Capacitance
L = Inductance
= Equivalent Series Resistance (ESR)
= Insulation Resistance (IR)
Where Z = Total Impedance
RS = Equivalent Series Resistance
XC = Capacitive Reactance = 2fCXL = Inductive Reactance = 2fL
RS + (XC - XL)2 2
DF = ESRXc
The variation of a capacitors impedance with frequencydetermines its effectiveness in many applications.
Dissipation Factor: Dissipation Factor (DF) is a mea-sure of the losses in a capacitor under AC application. It is theratio of the equivalent series resistance to the capacitive reac-tance, and is usually expressed in percent. It is usually mea-sured simultaneously with capacitance, and under the sameconditions. The vector diagram in Figure 2 illustrates the rela-tionship between DF, ESR, and impedance. The reciprocal ofthe dissipation factor is called the Q, or quality factor. Forconvenience, the Q factor is often used for very low valuesof dissipation factor. DF is sometimes called the loss tangentor tangent d, as derived from this diagram.
Insulation Resistance: Insulation Resistance (IR) is theDC resistance measured across the terminals of a capacitor,represented by the parallel resistance (Rp) shown in Figure 1.For a given dielectric type, electrode area increases withcapacitance, resulting in a decrease in the insulation resis-tance. Consequently, insulation resistance is usually specifiedas the RC (IR x C) product, in terms of ohm-farads ormegohm-microfarads. The insulation resistance for a specificcapacitance value is determined by dividing this product bythe capacitance. However, as the nominal capacitance valuesbecome small, the insulation resistance calculated from theRC product reaches values which are impractical.Consequently, IR specifications usually include both a mini-mum RC product and a maximum limit on the IR calculatedfrom that value. For example, a typical IR specification mightread 1,000 megohm-microfarads or 100 gigohms, whicheveris less.
Insulation Resistance is the measure of a capacitor toresist the flow of DC leakage current. It is sometimes referredto as leakage resistance. The DC leakage current may becalculated by dividing the applied voltage by the insulationresistance (Ohms Law).
Dielectric Withstanding Voltage: Dielectric withstand-ing voltage (DWV) is the peak voltage which a capacitor isdesigned to withstand for short periods of time without dam-age. All KEMET multilayer ceramic capacitors will withstand atest voltage of 2.5 x the rated voltage for 60 seconds.
KEMET specification limits for these characteristics atstandard measurement conditions are shown in Table 1 onpage 4. Variations in these properties caused by changingconditions of temperature, voltage, frequency, and time arecovered in the following sections.
KEMET Electronics Corporation, P.O. Box 5928, Greenville, S.C. 29606, (864) 963-6300 5
APPLICATION NOTES FOR MULTILAYERCERAMIC CAPACITORS
APPLICATION NOTES FOR MULTILAYER CERAMIC CAPACITORS
KEMET Electronics Corporation, P.O. Box 5928, Greenville, S.C. 29606, (864) 963-63006
TABLE 1EIA TEMPERATURE CHARACTERISTIC CODES
FOR CLASS I DIELECTRICS
Significant Figure Multiplier Applied Tolerance ofof Temperature to Temperature Temperature
Coefficient Coefficient Coefficient *
PPM per Letter Multi- Number PPM per LetterDegree C Symbol plier Symbol Degree C Symbol
0.0 C -1 0 30 G0.3 B -10 1 60 H0.9 A -100 2 120 J1.0 M -1000 3 250 K1.5 P -100000 4 500 L2.2 R +1 5 1000 M3.3 S +10 6 2500 N4.7 T +100 77.5 U +1000 8
+10000 9* These symetrical tolerances apply to a two-point measurement oftemperature coefficient: one at 25C and one at 85C. Some deviationis permitted at lower temperatures. For example, the PPM tolerancefor C0G at -55C is +30 / -72 PPM.
TABLE 2EIA TEMPERATURE CHARACTERISTIC CODES
FOR CLASS II & III DIELECTRICS
Low Temperature High Temperature Maximum CapacitanceRating Rating Shift
Degree Letter Degree Number LetterCelcius Symbol Celcius Symbol Percent Symbol
+10C Z +45C 2 1.0% A-30C Y +65C 4 1.5% B-55C X +85C 5 2.2% C
+105C 6 3.3% D+125C 7 4.7% E+150C 8 7.5% F+200C 9 10.0% P